Tear Strength Analysis of MDX4-4210 and A-2186 Silicones with Different Intrinsic Pigments Incorporated by Mechanical and Industrial Methods

Objective The aim of this study was to evaluate the tear strength of MDX4-4210 and A-2186 silicones with different intrinsic pigments incorporated by mechanical and industrial methods, comparing nonaged and aged groups. Materials and Methods Twenty-four groups were created according to the American Society for Testing and Materials D-624/type C, half nonaged and half aged (n = 10): bronze mechanical MDX4-4210, bronze industrial MDX4-4210, black mechanical MDX4-4210, black industrial MDX4-4210, pink mechanical MDX4-4210, pink industrial MDX4-4210, bronze mechanical A-2186, bronze industrial A-2186, black mechanical A-2186, black industrial A-2186, pink mechanical A-2186, and pink industrial A-2186. All specimens were submitted to tear strength analysis. Data were submitted to the ANOVA and Tukey test (p < 0.05). Results An increase in the tear strength values was observed only for the bronze and black MDX4-4210, comparing nonaged and aged silicones (p < 0.05), regardless of the manufacturing method. There was a difference in all comparisons between MDX4-4210 and A-2186 silicones with the same pigment type (p < 0.05), regardless of the manufacturing method. In all cases, there was no difference in the manufacturing method comparing the MDX4-4210 or A-2186 groups with the same pigment. Conclusion Accelerated aging did not influence the tear strength in all aged A-2186 silicones and in aged pink industrial and mechanical MDX4-4210 silicones. The other MDX4-4210 groups had an increase in the results after aging. In all cases compared, the A-2186 groups had higher tear strength values than the MDX4-4210 groups. Mechanical and industrial methods can be used for silicone preparation, without changing the tear strength.

ese are the most accepted materials due to the ease of handling, chemical inertia, proper strength, durability, biocompatibility [4,11,12], flexibility, texture similar to that of the human skin, and heat stability. Additionally, these materials repel water, blood, and organic materials, thus eliminating bacterial colonization [8]. e thin margins of silicone prostheses are usually glued to the patient's face using a medical adhesive. e thin margins of this type of prosthesis are susceptible to tearing as the prosthesis is removed from the attached facial tissue [4,6]. In addition, maxillofacial prostheses can be retained by implants. For this, a layer of acrylic resin is adhered to the silicone to facilitate the bonding of the silicone to the implant. However, there is no good chemical adhesion between the silicone and the resin, which can result in the tearing of the silicone during the removal of the prosthesis [7].
An increase in the tear strength of a silicone can promote an increase in the esthetic quality of the facial prosthesis since it allows the use of thinner margins, with greater possibility of elongation and lesser chance of rupture [4]. According to Rai et al. and Aziz et al., the most important property for maxillofacial prostheses is the tear strength, from a clinical point of view [4,6].
Silicone elastomers may be influenced by a variety of factors, such as intrinsic pigmentation [4], ultraviolet (UV) light [8,10], and/or the manufacturing method (pigment incorporation method into silicone) [13]. When the pigment is mixed with silicone, bubbles may be incorporated into the material.
ese bubbles may influence the mechanical properties (e.g., tear strength) of a silicone [13]. e method for incorporating pigment into silicone can help minimize bubble incorporation [13]. erefore, the study of methods of incorporating the intrinsic pigment to the silicone is very important for the durability of a facial prosthesis.
e Silastic MDX4-4210 is an elastomer widely used for facial rehabilitation [14][15][16]. In the studies of Dootz et al., Sanchez et al., and Haug et al., the tear strength of MDX4-4210 silicone is compared with that of A-2186 silicone [10,15,17]. However, these comparisons did not evaluate the incorporation of different pigments and/or different methods of manufacturing of these materials. erefore, the aim of this study was to evaluate the tear strength of MDX4-4210 and A-2186 silicones with different intrinsic pigments incorporated by mechanical and industrial methods, comparing nonaged and aged groups.

Materials and Methods
For this study, Silastic MDX4-4210 (Dow Corning Corporation Medical Products, USA) and A-2186 (Factor II, AZ, USA) silicones were prepared with the addition of intrinsic pigments. Bronze (Functional Intrinsic II-215, Factor II, USA) and black (Black Functional Intrinsic II-205, Factor II, USA) pigments specific for characterization of prostheses were used. In addition, a new pink pigment (Orbital Colors, Brazil) was tested. e pink pigment was formed by the union of yellow, red, and black pigments and white opacifier. All tested pigments had an organic origin and the white opacifier (TiO 2 ) had a mineral origin. e silicones and pigments were weighed on a digital analytical balance (Adventurer, Ohaus Corporation, USA). Each pigment from Factor II (bronze and black) corresponded to 0.2% of the weight of its respective silicone [2]. For the pink pigment, the pigments that constituted it corresponded to 0.6% (white) [18], 0.122% (yellow), 0.03% (red), and 0.006% (black) [2] of the silicone weight.
A total of 240 specimens were manufactured (Figures 1(a) and 1(b)). e silicones were manipulated according to each manufacturer's instructions at a temperature of 23 ± 2°C [2,8,9,12]. Half of the specimens were fabricated by the mechanical method of incorporating the intrinsic pigment to the silicone. For this, the pigment was manually mixed with the silicone for 15 seconds, followed by a vacuum spatulation at 425 rpm in a mechanical spreader (Polidental Ind. e Com. Ltda, Brazil) until the mass became homogeneous. Subsequently, the silicone was inserted into a metal matrix. e matrix was closed and submitted to 1 ton for 10 minutes. After this period, the silicone contained in the matrix was placed on a bench and exposed to the environment (29°C) for 72 hours, until the complete polymerization of the material. e other half of the specimens was fabricated at Orbital Colors using the industrial method of incorporating the intrinsic pigment to the silicone by means of a grinding machine (CHSG/3-Roll Mill, Chemieland, China). e pigment was mixed with the silicone in the machine. en, the silicone was inserted into the matrix, following the same procedure as the previous method. In this method, the Deutsches Institut für Normung (DIN-53235) was used. Specimens were made in matrices with standard dimensions and had a 2 mm thickness ( Figure 2).
Twenty-four groups were created, half nonaged and half aged (n � 10): bronze mechanical MDX4-4210, bronze industrial MDX4-4210, black mechanical MDX4-4210, black industrial MDX4-4210, pink mechanical MDX4-4210, pink industrial MDX4-4210, bronze mechanical A-2186, bronze industrial A-2186, black mechanical A-2186, black industrial A-2186, pink mechanical A-2186, and pink industrial A-2186. e specimens were submitted to the accelerated aging test using an accelerated aging chamber (Equilam, Brazil) according to the American Society for Testing and Materials-Designation G53-96) [19]. e lamps (UVB 313, 40 Watts, Equilam, Brazil) emitted UVB light at a wavelength of 313 nm and irradiation of 0.49 W/m 2 /nm. en, they were subjected to alternating periods of UVB light and condensation using oxygen-saturated distilled water, under conditions of heat and 100% humidity. Each aging cycle lasted 12 hours. In the first 8 hours, the temperature was maintained at 60 ± 3°C and the UV light was imputed onto the specimens. In the last 4 hours, the temperature was maintained at 45 ± 3°C and a condensation period occurred without light [2,3,8,11]. e aging was performed for a total of 1008 hours, and the deterioration caused by rain, dew, and UV light from the sun was simulated [2,3,8,11]. is period corresponded to approximately one year of prosthesis use [11]. e specimens that would not be aged were stored in a dark chamber at room temperature (23 ± 2°C) and 50 ± 5% relative humidity for 1008 hours [20].
All specimens were tested using a universal testing machine (EMIC, Instron, Brazil) ( Figure 3). Specimens were stretched at a rate of 500 mm/min. e maximum tear strength value was recorded in Newtons (N). e process was determined according to the American Society for Testing and 2 International Journal of Dentistry Materials (ASTM) D-624 (type C) [4,14,17]. e formula T � F/D was used, with F being the maximum force required to break the specimen and D being the thickness of the specimen. e results were obtained in N/mm. All data were analyzed using the Statistical Package for Social Sciences 20.0 (SPSS-IBM Corp., USA). e normal distribution was verified through the Shapiro-Wilk test. Data were analyzed through the analysis of variance (ANOVA) and the Tukey test, with a level of significance of 5%.

Results
Tables 1-5 show the mean and standard deviation (SD) of each group. In Table 1, the tear strength of nonaged and aged silicone groups with the same pigmentation was compared. ese comparisons were made within each manufacturing method. An increase in the tear strength values was observed only for the bronze and black MDX4-4210 silicone, for both manufacturing methods (p < 0.05). Table 2 shows all nonaged groups, comparing MDX4-4210 and A-2186 silicones, based on the same pigment type. ese comparisons were made within each manufacturing method. e tear strength values were higher for the A-2186, compared with the MDX4-4210 silicone (p < 0.05). Table 3 shows all aged groups, comparing MDX4-4210 and A-2186 silicones, based on the same pigment type. ese comparisons were made within each manufacturing method. In all cases, the tear strength values were higher for the A-2186, compared with the MDX4-4210 silicone (p < 0.05). International Journal of Dentistry Table 4 shows all non-aged groups, comparing the mechanical and industrial methods, within the MDX4-4210 and A-2186 groups, with the same pigment type. ere was no difference between the manufacturing methods (p > 0.05). Table 5 shows all aged groups, comparing the mechanical and industrial methods, within the MDX4-4210 and A-2186 groups, with the same pigment type. ere was no difference between the manufacturing methods (p > 0.05).

Discussion
In this study, it was possible to observe a statistically significant increase in the tear strength of aged bronze and black MDX4-4210 silicone, for both manufacturing methods, when compared with the respective nonaged groups. ese results show that there was an increase in the tear strength of this silicone, regardless of the pigment color (lighter or darker). Presumably, the polymerization of this material was incomplete after its manufacture, and the UV light continued this process [8]. Despite this, there was no increase in this property for aged pink industrial and mechanical MDX4-4210 groups (Table 1).
is could have occurred because the new pink pigment has TiO 2 in its constitution. is component has a high refractive index and is used in the manufacture of sunscreens to protect human skin against UV rays [8,11,18]. erefore, the TiO 2 must have prevented UV rays from influencing the polymerization of pink industrial and mechanical MDX4-4210 groups.
For the A-2186 groups, regardless of the pigment or manufacturing method, there was no significant statistical difference in tear strength comparing nonaged and aged groups (Table 1). is suggests that the polymerization of this silicone has been complete since its manufacture. erefore, the UV rays had an insignificant influence on the same.
Regardless of the manufacturing method, the A-2186 silicone showed significantly higher tear strength values compared with the MDX4-4210 silicone, when the same pigment was used (Tables 2 and 3). is difference could have occurred due to the higher filler loading and/or higher molecular weight of the dimethylsiloxane polymer from the A-2186 silicone [16]. Despite using different methodologies, this result corroborates the studies performed by Dootz et al. [10], Sanchez et al. [15], and Haug et al. [17]. According to Sanchez et al., higher values of tear strength of the A-2186 silicone compared with the MDX4-4210 silicone may clinically indicate higher prosthesis longevity [15].
When comparing mechanical and industrial methods for each silicone with the same pigment, there was no statistically significant difference (Tables 4 and 5). is may have occurred because these methods generated a similar homogeneous mixture between the silicone and pigment, with     International Journal of Dentistry 5 for the patient. erefore, the use of the mechanical method can be more economically advantageous and faster. is study had the limitation of the evaluation of only one property (tear strength) in the facial silicones. erefore, there is a need for other studies evaluating other properties.

Conclusion
Accelerated aging did not influence the tear strength in all aged A-2186 silicones and in aged pink industrial and mechanical MDX4-4210 silicones. e other MDX4-4210 groups had an increase in the results after aging. In all cases compared, the A-2186 groups had higher tear strength values than the MDX4-4210 groups. Mechanical and industrial methods can be used for silicone preparation, without changing the tear strength.

Data Availability
e data used to support the findings of this study are included within the article.